Alternate Names: Roasted Alberta Slip
Fully calcined Alberta Slip (fired at 1900F) has an LOI of 9%. However it is not necessary to fire it that high to remove the plasticity (to reduce shrinkage during drying). The albertaslip.com website outlines this 1000F roasting process. This version looses only 3% of its weight on firing, so the analysis totals 97.
Roasted Alberta Slip (right) and raw powder (left). These are thin-walled 5 inch cast bowls, each holds about one kg. I hold the kiln at 1000F for 30 minutes. Why do this? Because Alberta Slip is a clay, it shrinks on drying. Roasting eliminates that, a 50:50 raw:roast mix works well for most recipes having high percentages of Alberta Slip. And 1000F? Calcining to 1850F sinters some particles together (creating a gritty material) while 1000F produces a smooth, fluffy powder. Technically, Alberta Slip losses 3% of its weight on roasting so I should use 3% less than a recipe calls for. But I often just swap them gram-for-gram.
This high-Alberta-Slip glaze is shrinking too much on drying. Thus it is going to crawl during firing. This common issue happens because there is too much plastic clay in the glaze recipe (common with slip glazes). Clay is needed to suspend the other particles, but too much causes the excessive shrinkage. The easiest way to fix this is to use a mix of raw and calcined Alberta Slip (explained at albertaslip.com). The calcined Alberta Slip has no plasticity and thus much less shrinkage (but it still has the same chemistry). Many matte glazes have high kaolin contents and recipes will often contain both raw and calcined kaolin for the same reason.
|Materials||Alberta Slip 1900F Calcined|